The Effect of Macromonomer Surfactant Microstructure on Aqueous Polymer Dispersion and Derived Polymer Film Properties

Water-borne coatings were prepared from poly(methyl methacrylate-co-butyl acrylate) latexes using different methacrylic acid containing macromonomers as stabilizers, and their physical properties were determined. The amphiphilic methacrylic acid macromonomers containing methyl, butyl, or lauryl methacrylate as hydrophobic comonomers were synthesized via catalytic chain transfer polymerization to give stabilizers with varying architecture, composition, and molar mass. A range of latexes of virtually the same composition was prepared by keeping the content of methacrylic acid groups during the emulsion polymerization constant and by only varying the microstructure of the macromonomers. These latexes displayed a range of rheological behaviors: from highly viscous and shear thinning to low viscous and Newtonian. The contact angles of the resulting coatings ranged from very hydrophilic (<10°) to almost hydrophobic (88°), and differences in hardness, roughness, and water vapor sorption and permeability were found.


■ INTRODUCTION
Colloidal polymer particles have been studied over the past several decades, and their applications have received an increasing attention in various fields, ranging from various biomedical applications, such as medical imaging, 1 drug delivery systems, 2−7 biosensors, 8−10 biofilms, 10−12 and antibacterial coatings, 12−16 and applications such as pressure sensitive adhesives 17−19 and protective 20−23 and antifouling coatings. 24,25These colloidal polymer particles are often synthesized via emulsion polymerization and can be functionalized using dedicated monomers and surfactants.−28 In general, most used surfactants are not covalently bound to the colloidal particles and can diffuse from the particles into the environment or from the bulk to the film surface (and potentially desorb).−68 These macromonomers were composed of methacrylic acid (MAA) and methyl methacrylate (MMA), butyl methacrylate (BMA), lauryl methacrylate (LMA), or butyl acrylate (BA) and used in the emulsion polymerization of methyl methacrylate and/or butyl acrylate.By varying the composition, chain length, and concentration of the macromonomers, we were able to tune the particle size, molar mass, and rheological behavior of the latexes.We found that pMMA latexes were best stabilized by statistical MAA macromonomers containing BMA and LMA as comonomers, and these latexes showed a small yield stress and shear thinning behavior, properties which are useful for binders in, e.g., waterborne paints. 69n this work, we selected earlier synthesized macromonomers with different architectures and compositions to prepare latexes and coatings to investigate the influence of the used macromonomer structure on the latex and film properties while keeping the amount of MAA groups (0.025 mol) of the macromonomer and the overall latex composition constant.Although the systems we investigate are not directly aimed at biomedical applications, we expect the results to be of general relevance to any emulsion polymerization using reactive polymeric surfactants.
■ EXPERIMENTAL SECTION Materials.MMA and BA were obtained from Sigma-Aldrich (99%) and passed over a column of inhibitor remover (Sigma-Aldrich).Potassium persulfate (KPS, p.a.) and sodium carbonate (dehydrated, p.a.) were purchased from Merck and used as received.Macromonomers were synthesized and characterized as part of previously published work, 66−68 and their main characteristics are summarized in Table 1.

Preparation of Latexes.
Emulsion polymerizations were carried out under an argon atmosphere in a standard 250 mL baffled jacketed thermostated glass reactor, equipped with a mechanical four-bladed turbine stirrer.For semibatch emulsion polymerizations, the reactor was charged with 75 g of deionized water, buffer, macromonomer, and 5 g of monomers (i.e., 9 wt % of the overall monomer content), stirred at 360 rpm, purged with argon for 30 min, and subsequently heated to 60 °C (see Table 2 for the standard recipe).Five minutes after reaching a constant temperature, a 4.1 × 10 −3 M aqueous KPS solution (10 mL of water containing 0.1 g of KPS) was injected to start the polymerization.
Starting 1 h after initiation, the temperature was raised to 70 °C to increase the polymerization rate, and the remaining monomer (50 g) was added at a constant feeding rate of 4−5 mL h −1 , resulting in starved-feed conditions.The mixture was left to react overnight (24 h) to maximize the final conversion; conversions of the monomers were determined gravimetrically.The resulting polymers were characterized using size exclusion chromatography (SEC), differential scanning calorimetry (DSC), and dynamic vapor sorption (DVS).The latexes were characterized using dynamic light scattering (DLS) and scanning and transmission electron microscopy (SEM, TEM) for particle sizes and distributions, electrophoresis for zeta potentials, and rheometry for viscosity and dynamic moduli measurements.For details of these characterization techniques, see the Supporting Information (SI).
Preparation of Coatings.Thin films were cast directly from the latex onto a glass substrate using a doctor blade applicator with an opening of 120 μm fixed in an application device, which moved at a constant speed of 10 mm/s.The films were dried overnight at either 20 or 40 °C.After drying, the films were annealed at 60 °C for 5 days.Thick films for DVS analyses were prepared by casting latex in an aluminum mold and drying in a vacuum oven at 60 °C for 5 days, and thick films for dynamic mechanical analysis (DMA) were prepared by casting latex in a Teflon mold and drying at room temperature.The surfaces of all films were examined visually and investigated by atomic force microscopy (AFM) and SEM.Physical properties of the thin films, such as contact angle and interfacial tension, were measured using an OCA15Pro goniometer.Additionally, the Konig hardness, cross hatch adhesion, and gloss of these coatings were measured.For details of these characterization techniques, see the Supporting Information (SI).

■ RESULTS AND DISCUSSION
We will first discuss the emulsion polymerization, followed by a discussion of the characterization of the latexes, emulsion polymers, and polymer films.

Synthesis and Analysis of Latexes and Emulsion Polymers.
Latexes with an overall solids content of ∼40% were prepared using the different methacrylic acid macromonomers from Table 1 with a constant amount of MAA units in the reactor (0.025 mol).A typical graph of the overall monomer conversion and total amount of monomer fed for the starved-feed polymerizations is shown in Figure 1a.From this graph, it can be seen that during the seed stage (i.e., the first hour at 60 °C), the polymerization rate first increases rapidly, then levels off (see SI for more details), is constant during the following feed stage, and finally decreases due to a decreasing monomer concentration.The polymerization was started at 60 °C to have a comparable temperature during the seed stage as in our previous work; 66−68

Biomacromolecules
maintain starved-feed conditions during the entire polymerization.All polymerizations reached a final conversion of at least 99% overnight.The polymerizations using relatively hydrophilic surfactants show a low polymerization rate during the seed stage of the reaction; these curves are shown in Figure 1b.−68 However, in most cases, the usual polymerization rates were reached again after some induction time, except for the polymerization with the h-MAA 350 macromonomer, which needed a seed time of more than 8 h.In all cases, no significant coagulation ( ̃irreversible aggregates) was observed after the polymerization, except for some minor coagulation around the stirrer and on the reactor wall (<3 wt %).As in our previous work, 66−68 we categorized the latexes according to their visual appearance into three types to facilitate the further discussion: type I is a colloidally stable liquid-like latex (low viscosity, containing no visible sediment/ coagulum), type II is a (weakly) redispersible, flocculated latex, and type III is a highly viscous latex with a strong internal physical network structure and behaves like a solid in rest.
We determined the particle size distributions of the latexes using different techniques: DLS, SEM, and TEM.Furthermore, the zeta potential (ζ) of all latexes was measured at pH = 10 and for all latexes ζ and hydrodynamic diameter (D H ) were measured as a function of pH.For the nomenclature of the latexes and their characteristics, see Table 3 (see the SI for PSD and the pH-dependence of D H for each latex).Typically, for the type II and III latexes (sL l , sB l , hA l , and hA s ), we observed broad particle size distributions (PSD) and high hydrodynamic diameters using DLS, (e.g., D H for sL l ≈ 2100 nm), with D H being much larger than the number-averaged (D n ), volume-averaged (D v ), and intensity-averaged (D I ) diameters.The results for type III latex (sL l ) are shown in Figure 2.
For the type I latexes, the PSD is in general narrower, and the hydrodynamic diameters (e.g., D H for bM ≈ 120 nm) are only slightly larger than the average diameters (D n , D v , and D I ).The small increase in D H compared to D n measured using DLS, SEM, or TEM is due to swelling of carboxylic groups at the surface of the latex particles. 70The results for a typical type I latex: bM are shown in Figure 3.
Since the D n values determined from the SEM and TEM images (D n,SEM and D n,TEM ) are comparable to the D n calculated from the DLS measurements (D n,DLS ), we will use the D n values to compare the particle sizes of the different latexes.When we look at the D n,SEM of all latexes, it is clear that these are the smallest in the case of bM and sL s and are comparable to the particle diameter of the reference SDS latex (LSDS) (∼75 nm).hA l has the largest particle diameter (∼1200 nm); in this case, a long macromonomer consisting of only MAA was used and the time to form (micelles and) primary particles was long (>8 h) (see Figure 1b), and so finally fewer and therefor larger particles were formed.
Considering all latexes, we see large differences in the D H (in Table 3).D H is a measure of the particle diameter in the water phase, including the shell of stabilizing surfactants absorbed or anchored on the particle surface and the hydrophilic chains extended into the water phase.To investigate this shell of surfactant molecules, we measured ζ and D H as a function of the pH from basic (pH = 10) to acidic (pH = 2); for each latex a plot of D H as a function of pH is shown in the SI.By reducing the pH, the charge of the anionic (MAA) groups in the surfactant will be neutralized, the shell, if present, will collapse, and the electrosteric stabilization will be reduced.This will result in a decrease (of the absolute value) of ζ and potentially an increase of D H, when particles agglomerate into larger flocs.At low pH (pH < 4), we see a large decrease of the (absolute) value of ζ for most latexes.Only bM shows no influence at all on both ζ and D H , which is more comparable to LSDS.Also, for sL s , D H is constant from pH = 10 to pH = 2.5, although ζ is gradually decreasing.This lack of influence of the pH on D H suggests that the surfactants in these three latexes are not extending from the particle surface into the water phase but stay more on the surface. 71The influence on D H for sL l , sB l , sM l , and hA l could not be investigated because D H was above or close to the measurement threshold of the instrument.This high D H is caused by large chains extending from the surface into the water phase, thus forming a strong internal network.This steric stabilization not only increases the hydrodynamic size of the particles but also increases the low shear viscosity (η min ) of the latex and results in a shear thinning latex (see below). 71,72The presence of these extending chains (or hairy structures) was confirmed by cryo-TEM (Figure 4), and small

Biomacromolecules
features interrupting the under focus rings are visible (for higher magnification and more details see the SI, Figure S15).
In general, we can say that latexes with a larger steric component (sL l , sB l , sM l , and hA l ) show a higher D H and a lower ζ compared to the latexes stabilized by the shorter macromonomers (sL s , sB s , sM s , and hA s ).
To get a more quantitative insight into the rheological properties of the prepared latexes, we measured the steady state viscosities as a function of the shear rate (Figure 5a) and performed a dynamic time sweep for a period of 1000 s to probe the mechanical microstructure to determine the dynamic moduli G′ and G″.To check the recoverability of the structure after such a time sweep, the sample was stirred (using a shear rate of 100 s −1 for a duration of 100 s), after which another dynamic time sweep was recorded (Figure 5b).In Figure 5, typical results of the viscosity measurements and the dynamic time sweep experiments are shown for all types of latexes (for details of all latexes, see the SI).Type I latexes show a typical Newtonian behavior: viscosities are independent of the shear rate (Figure 5a) and these latexes show liquid-like behavior (G″ ≫ G′, Figure 5b).Both type II and III latexes show clear shear thinning behavior, although the viscosities of type III are higher than those of type II over the full range of shear rates; accordingly, the storage and loss moduli of types II and III are also higher than those of type I. sL l is the only type III latex.Both sL l (type III) and sB l (type II) show G′ > G″, indicating viscoelastic solid-like behavior (see Figure 5b).The other type II latexes, hA l and hA s , also show high values for G′, but G′ < G″, so their behavior is more liquid-like (see the SI for details).
High values of G′ and G′ > G″ for type II and III latexes indicate the presence of strong internal structures, which can be broken up by stirring, but after stirring are immediately restored to the same level (see Figure 5b).These four latexes show clear shear thinning behavior and at high shear rates the viscosities tend to level off, suggesting that the internal structures are no longer broken up by increasing shear rates; the leveling off takes place at relatively high viscosities suggesting that large agglomerates or flocs with strong interactions still exist. 29Also, sL s and bM (both type I) show shear thinning, but at much lower viscosities, and already at shear rates of >0.01 s −1 , the viscosities level off (η max ≈ 1 × 10 −2 Pa•s).All these shear thinning latexes show a slope of around −1 in a double-log plot, indicative of plastic behavior; this means that large agglomerates stick to each other and form soft solids with stresses, τ min , ranging from ∼20 (for sL l ) to ∼4 × 10 −4 Pa (for sL s and bM) at the lowest measured shear rate (γ̇= 0.001 s −1 ) (see Table 3 and Figure S17).The internal network at rest or a low shear rate is caused by the interaction of charged polymer chains present on the particle surface at the high pH values of the latexes.These anionic charges will repel each other, and the polymers swell and uncoil occupying more volume within the water phase.Additionally, the hydrophobic groups present can form domains along other hydrophobic groups giving a more structured, less liquid-like system. 73The other four latexes (sB s , sM l , sM s , LSDS) showed very low and almost constant viscosities (η ≈ 1 × 10 −2 Pa•s) at increasing shear rates (Newtonian) and no (yield) stresses were measurable; this liquid-like behavior was confirmed by the dynamic measurements (G" ≫ G′; G′ ≈ 0).
Next, we characterized the polymers synthesized in the emulsion polymerizations.In   Biomacromolecules bulk polymer measured using DVS are listed (see details per latex in the SI).In general, the values for T g measured using DSC were only slightly different from those estimated using the Fox equation 74 and slightly higher than the T g of the reference emulsion polymer (LSDS), because of the incorporation of the (higher T g ) macromonomer in the polymer chains.For sL l , we see a broad glass transition; here, copolymers were formed with different built-in amounts of (macro)monomer, probably caused by diffusion limitations at the end of the polymerization due to the high viscosity of this latex.
The SEC results in Table 4 show very broad molar mass distributions irrespective of the used stabilizer.It is known that although the macromonomers can function as chain transfer agents, they will undergo complex copolymerization 49 during the emulsion polymerization and can be buried inside the polymer particles.The resulting polymers are characterized (using DMA) by a relatively constant rubbery plateau (G 0 ) between ∼0.5 and ∼1 MPa as is clear from Table 4.
Finally, dynamic water vapor sorption analyses were performed for all 10 polymers.The equilibrium relative humidity (RH) in the cell was varied from 0.5% (i.e., the dry state) to 95% (i.e., the wet state) and back to 0.5% with steps of 5−10%.The change in mass of the polymer at each RH was measured constantly, and after reaching equilibrium (dm/dt < 0.005 wt %/min), the RH was increased (sorption) or decreased (desorption) to the next value.The results for a typical sorption−desorption experiment are shown in Figure 6 for the reference latex LSDS.
Typically, we see an increase of the mass when the RH increases and a decrease of the mass when the RH decreases.The gap between the sorption and desorption isotherms in Figure 6b is indicative for bulk sorption/desorption. 75 The isotherms of all other emulsion polymers are plotted in Figure     Latex properties listed in Table 3. b T g calculated with the Fox equation, 74 (see eq 1 in SI) using measured T g s of macromonomers listed in Table 1.c Storage modulus at rubbery plateau.the SI for results of all preparations).For adhesion and gloss measurements, latex films were cast onto an aluminum substrate and dried at 20 °C overnight (prep A only).The surfaces of all prepared films were examined visually and imaged using AFM and SEM.Furthermore, physical properties such as roughness, hardness, cross hatch adhesion, and gloss were determined.Additionally, the contact angles of the coatings and the interfacial tensions of water droplets on the surface of the coatings were measured using goniometry and the diffusion coefficients and permeabilities for water vapor were determined by DVS.The physical properties of the films are summarized in Table 5.
−84 As an example for a clear coating, the AFM and SEM images of sL s are shown in Figure 8. From the AFM images (Figure 8a,b), it can be seen that the surface is rather homogeneous, only some larger (flattened) particles (height ≈ 20 nm) are visible, and the average roughness (R a ) of the surface is only 4 nm; an R a ≤ 4 nm is considered smooth. 85Additionally, SEM (Figure 8c) of the same film showed a smooth surface.Latex properties listed in Table 3. b Prep A (A): film dried at 20 °C, prep D (D): film dried at 40 °C and annealed at 60 °C.c R a is roughness of the surface at an evaluation length of 5 μm measured using AFM.d Oscillating time measured according to ASTM 4356. 79e Gloss values (in gloss units (GU)) and % reflection at 85°. f Cross hatch adhesion measured according to ASTM 3359 80 scale from 5B (no damage) to 0B (fully detached).g Water contact angle measured via sessile drop method, γ lg is the water−air interfacial tension of a water droplet from the coating surface measured via pendant drop method, 81 and γ lg of water in air is 72.1 mN•m −1 .h Diffusion coefficient (D dif ) and permeability (P) of water vapor through a thick film using a Payne cell. 82i Not measured.
When we analyze one of the hazy films, e.g., sM l (prep A), using SEM (Figure 9a), we see areas showing closely packed large particles (>1 μm).Zooming in at other areas (Figure 9b), we also see large particles but now surrounded by many small particles (∼120 nm); this is also observed in the DLS data measured directly after polymerization (see SI), implying that the large particles were formed during polymerization.The presence of smaller particles is desirable to improve the film formation by increasing the capillary forces needed for coalescence. 86,87These large particles surrounded by smaller ones are also observed using AFM (Figure 9c,d) and in AFM and SEM for some of the other coatings (sL l , sM s , and hA l ); all these coatings contain a high T g macromonomer (see SI for AFM images of the other films).When considering the SEM image in more detail, we observe that these large particles seem to be hollow (see some broken particles in the SEM image in Figure 9b).A similar observation was previously described in the literature for core−shell particles with different T g values in the core and shell using (meth)acrylic acid as a comonomer and was ascribed to the soft BA/MMA core flowing out of the hard MMA shell. 85Something similar could also have happened in our case and if these large particles contain water or air; this inclusion can result in hazy or opaque films, 86,87 which is also observed for films from sL l , sM l , and hA l .To improve the appearance of the hazy films (i.e., sL l , sM l , and hA l ), the films were annealed at 60 °C (prep D) and even 100 °C for 5 days.This resulted in a clear film for sM l but not for sL l and hA l ; therefore, these two coatings were not investigated further.
Using AFM, we also analyzed the roughness of the films prepared by using different drying methods.We observed that drying the films at 40 °C (prep B) instead of 20 °C (prep A) does not have a large influence on the roughness; due to the decreased drying time at higher temperatures, the particles have less time to coalesce.Annealing of both films at 60 °C (preps C and D) decreased the roughness significantly (see Table 5).All clear coatings appear to have a roughness (R a ) that is lower than that of the reference coating (LSDS).
We also measured the gloss, hardness, and adhesion of the coatings using prep A and compared these results with those of the reference coating LSDS (Table 5).The very low roughness of all coatings results in high gloss (i.e., gloss values >80 GU 88 ); all films except for hA s show gloss values of >87 GU.Cross hatch adhesion of the different coatings, except those of bM and hA s , was better than that of LSDS.For the films of sL s , sB l , and bM, the measured hardness values are higher than for LSDS.The coating with the highest T g (sB l ), which is also just above the measuring temperature (T ≈ 19 °C), appears to be also the hardest, and we see that the surfactants with the shortest chains (sB s, sM s , bM, hA s ) give the most damping (less oscillations) and thus appear to be the softest.
The presence of hydrophilic groups, such as MAA, at the surface of coatings is expected to have a large influence on the surface properties, so we will also discuss some relevant important physical properties, of the coatings: the water contact angle and interfacial tension of the surface, the diffusion coefficient, and the permeability of the film for water vapor.The water contact angle and the interfacial tension of water droplets on the surface (γ lg ) were measured using goniometry and the results are also listed in Table 5.Since all contact angles are below 90°, we can conclude that all coatings are hydrophilic.The hydrophilicity of the films decreases (increase of contact angle) in most cases when the films are dried at a higher temperature and after annealing.In most cases, the coatings are more hydrophobic than the reference LSDS coating, which was not immediately expected, especially because the number of acid groups in MAA (0.025 mol) in the reaction is 10 times higher than the number of hydrophilic sulfate groups of SDS (0.002 mol).The contact angles of coatings prepared using the longer macromonomers (sL l , sB l , sM l , and hA l ) are higher than those of the coatings prepared using the shorter chain analogues (sL s , sB s , sM s , and hA s ).The short macromonomers, which lead to better electrostatic stabilization of the latex particles (higher ζ potential), are located more at the surface of the particles and after drying also make the coating surface more hydrophilic.To determine whether the initial macromonomers are covalently bound to the polymer particles, we measured the interfacial tension (γ lg ) of a water droplet originating from the coating surface.For sL l , sL s , and bM, we see no change in the interfacial tension compared to pure water (γ lg for water−air is 72.1 mN•m −1 ), so no surface-active molecules were dissolved from the coating surface.The coatings prepared from sB s , sM l , sM s , hA l , and hA s gave a decrease of the γ lg , and in the case of sB s , sM l , and sM s , the water droplet also became white, indicating that molecules from the surface dissolved into the water droplet.A further indication that this is indeed the case is the observation that the supernatants of these latexes also contained water-soluble polymers (see SI, Figure S22 for SEC analyses of these supernatants).We also measured whether the presence of MAA groups has an influence on the diffusion coefficient (D Dif ) and the permeability (P) of the coatings for water vapor.The thickness of the films was around 500 μm.We measured the mass change as a function of time using a Payne cell with DVS for all coatings (see Table 5 for D Dif and P values and see the SI for the used equations and absorption curve).From the absorption curves, it could be concluded that the sorption of water vapor through the films is Fickian.All diffusion coefficients are between 1.5 × 10 −7 and 1.4 × 10 −8 cm 2 •s −1 and the permeabilities between 2 and 17 g•h −1 •m −2 •mm.The coatings with the lowest contact angles (highest hydrophilicity) show a slightly higher D Dif and P for water vapor than the less hydrophilic coatings.−91 The presence of MAA groups on the surface can increase the initial absorption of water at high RH (RH > 60%) and, through the hydroplasticization effect, increase the permeability. 78,92,93At lower humidity (RH < 50%), the permeability is more controlled by temperature and concentration differences over the two sides of the film, and the absorbed water molecules in the hydrophobic polymer will be more clustered and not contribute to the permeability. 78,91,92,94CONCLUSIONS In this work, we prepared coatings from latexes synthesized with BA and MMA stabilized with methacrylic acid (MAA) containing macromonomers having different architectures and compositions.Although we kept the overall composition of the monomers in the emulsion constant and used equal amounts of MAA in each emulsion polymerization, we obtained latexes and coatings with rather diverse properties, which allow tuning for particular applications.For example, very low water permeabilities are obtained for sL s , whereas a higher permeability is obtained for sB s .In construction applications, the former is required for corrosion protection, 21 whereas the latter is required for wood protection.We have also seen that coatings of different hardnesses can be obtained, which may also be important for certain cell-surface interactions.Small differences in the macromonomer microstructure were also found to affect the colloidal and rheological properties of the polymer latexes.The relatively high solids contents in these studies may not always be directly relevant for biomedical applications, but what causes the observed differences are the differences in "hairiness" of the particles, and this is of obvious importance in diagnostic and therapeutic application of polymer particles as a hairy layer around the particles will affect the interactions of the particles with their environment and with other molecules.For the application of a coating, the viscosity of the latex during and after application is also of obvious importance.Some of our latexes show shear thinning behavior at different viscosity levels, and others are more Newtonian.For example, sL s is a shear thinning latex with a small yield stress, which resulted in a high gloss, clear coating, which was hard and smooth, proved to have good adhesion on aluminum, and showed a low water permeability.Finally, we conclude that only relatively minor changes in the microstructure of reactive polymeric surfactants may lead to a large range of particle and film properties and that it is worthwhile to investigate these small changes in any system of interest.

* sı Supporting Information
The Supporting Information is available free of charge at https://pubs.acs.org/doi/10.1021/acs.biomac.4c00292.Detailed experimental details of the characterization techniques, summaries of all characterization results for each latex/coating, comparisons of DLS data, additional AFM results, additional SEM and cryo-TEM images, additional rheological data, contact angles, comparison of DVS sorption plots, additional kinetic plots of the emulsion polymerization, and SEC data of the supernatants of the produced latexes (PDF) ■

1 a
Macromonomer characteristics as listed in

Figure 2 .
Figure 2. Overview of results from DLS and SEM of a typical type III latex: sL l ; (a) PSD: intensity weighted (−); volume weighted (..) and number weighted (--) calculated using the CUMULANT model; (b) SEM image of diluted latex; (c) zeta potential (triangle up solid) and D H (circle solid) as a function of the pH of diluted latex, which is adjusted to pH = 10 with 0.1 M NaOH solution and titrated with 0.01 M HCl solution; the horizontal blue line at D H = 10 4 nm (10 μm) indicates the upper instrument measuring threshold for particle sizes.

Figure 3 .
Figure 3. Overview of results DLS and SEM of a type I latex: bM, (a) PSD: intensity weighted (−); volume weighted (..) and number weighted (--) calculated using the CUMULANT model, (b) SEM image of diluted latex; (c) zeta potential (triangle up solid) and D H (circle solid) as a function of the pH of diluted latex, which is adjusted to pH = 10 with 0.1 M NaOH solution and titrated with 0.01 M HCl solution; the horizontal blue line at D H = 10 4 nm (10 μm) indicates the instrument measuring threshold for particle sizes.

Figure 4 .
Figure 4. Cryo-TEM images of (a) sB l ; (b) sM l , and (c) sM s with hairy features visible on the surface.

Figure 5 .
Figure 5. Rheology of p(MMA-co-BA) latex according to type: type I: liquid-like, sM s ; type II: viscous latex with reversible flocculation, sB l ; type III, gel-like latex, sL l ; (a) steady state viscosity as a function of shear rate; (b) storage modulus G′ (solid line) and loss modulus G″ (dotted line) as a function of time.
d Number-average (M n ) and weight-average (M w ) molar mass determined by SEC (using THF) relative to polystyrene standards.e Water absorption = (M 95 − M 0 )/M 0; M 95 and M 0 are sample masses measured at 95% and 0.5% RH, respectively.f No adequate film formation.

Figure 6 .
Figure 6.(a) Water vapor sorption kinetics for LSDS as a function of the relative humidity (RH) in time.The black line is the change in sample mass during the first sorption and subsequently desorption.The red line is the RH in the cell; (b) water vapor sorption isotherm for LSDS as a function of RH, lower (solid) curve corresponds to absorption, and upper (dashed) curve to desorption.

Figure 7 .
Figure 7. Water sorption isotherms for the different emulsion polymers p(MMA-co-BA) as a function of the partial water vapor pressure or relative humidity (RH) over a range from 0 to 95%.The lower (solid) curve indicates absorption, and the upper (dashed) curve desorption.

Figure 8 .
Figure 8. AFM and SEM images of sL s ; (a) AFM height and (b) phase image of a film (prep A); (c) SEM image of a dried film (prep A), coated with 10 nm gold before imaging, bar 1 μm.

Figure 9 .
Figure 9. AFM and SEM images of sM l ; (a) SEM image of an area showing closely packed large particles; (b) SEM image showing an area with ∼1 μm particles surrounded by ∼120 nm polymer particles, the arrow points toward a broken particle; (c) AFM height and (d) phase image of a film (prep A).SEM images were prepared from a diluted latex, dried at 20 °C, and coated with 10 nm gold before imaging.
after 1 h, the reactor temperature was increased to 70 °C to obtain a faster polymerization rate to

Table 2 .
Standard Recipe of a Semi-batch Emulsion Polymerization of MMA and BA Using Different MAA (co)-Macromonomers as Surfactants b

Table 4 ,
average molar masses determined by SEC, glass transition temperatures (T g ) determined by DSC and DMA, and water absorption of the

Table 3 .
Characteristics of Synthesized Latexes Stabilized by MAA n -Based Macromonomers with Constant Added Amount of MAA in Reactor (0.025 mol) a Table1and recipe emulsion polymerization according to Table2; more detailed results for each latex can be found in the SI.
b Subscript "l" denotes a latex prepared with a relatively large and "s" a relatively short macromonomer.c Added mass of macromonomer or SDS relative to the total amount of added monomer.d Number-average diameter determined by respectively DLS (standard model CUMULANT, $ used model CONTIN), SEM, and TEM. e D H by DLS.f ζ-potential in diluted sodium carbonate solution (ca.0.01 wt %) at pH = 10.g Visual appearance of latex: type I: liquid-like latex, type II: weakly flocculated latex, type III: gel-like latex, 67 # (some) sedimentation in time.h Pa and n.a.means too low to be give reliable value.i Behavior under shear: ST = shear thinning; N = Newtonian.

Table 4 .
Characteristics of Synthesized Emulsion Polymers a a

Table 5 .
Physical Properties of Polymer Films a Prepared with Different Preparation Methods (Prep A and/or Prep D) b